#------------------------------------------------------------------------------
#$Date: 2016-03-24 03:08:50 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179615 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/79/4507954.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4507954
loop_
_publ_author_name
'Wei, Jingjing'
'Yang, Lu'
'Ma, Pengtao'
'Wang, Jingping'
'Niu, Jingyang'
_publ_section_title
;
 A Series of Multi-Dimensional Lanthanide-Containing
 Peroxoisopolymolybdates
;
_journal_issue                   8
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              3554
_journal_paper_doi               10.1021/cg400536e
_journal_volume                  13
_journal_year                    2013
_chemical_formula_sum            'Ce6 H115 Mo29 N3 Na2 O158'
_chemical_formula_weight         6354.89
_chemical_name_systematic
;

 ?

;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   notdet
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 123.8830(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   37.146(2)
_cell_length_b                   16.6971(11)
_cell_length_c                   28.400(3)
_cell_measurement_reflns_used    9829
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.13
_cell_measurement_theta_min      2.21
_cell_volume                     14623(2)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0287
_diffrn_reflns_av_sigmaI/netI    0.0319
_diffrn_reflns_limit_h_max       44
_diffrn_reflns_limit_h_min       -41
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -33
_diffrn_reflns_number            37119
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.82
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    4.352
_exptl_absorpt_correction_T_max  0.5249
_exptl_absorpt_correction_T_min  0.3277
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.885
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             11940
_exptl_crystal_size_max          0.33
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.17
_refine_diff_density_max         1.487
_refine_diff_density_min         -1.020
_refine_diff_density_rms         0.203
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.094
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     956
_refine_ls_number_reflns         12798
_refine_ls_number_restraints     66
_refine_ls_restrained_S_all      1.098
_refine_ls_R_factor_all          0.0464
_refine_ls_R_factor_gt           0.0415
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0368P)²+544.0206P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1064
_refine_ls_wR_factor_ref         0.1084
_reflns_number_gt                11565
_reflns_number_total             12798
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg400536e_si_002.cif
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               4507954
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ce1 Ce 0.091715(15) 0.67250(3) 0.36584(2) 0.01652(11) Uani 1 1 d .
Ce2 Ce 0.003560(15) 0.99264(3) 0.36327(2) 0.01546(11) Uani 1 1 d .
Ce3 Ce 0.252446(17) 1.20141(3) 0.30696(2) 0.02408(13) Uani 1 1 d .
Mo1 Mo -0.03406(2) 0.61420(4) 0.30341(3) 0.01538(16) Uani 1 1 d .
Mo2 Mo -0.09463(3) 0.47323(5) 0.29703(3) 0.02109(17) Uani 1 1 d .
Mo3 Mo -0.15429(3) 0.61925(5) 0.28509(3) 0.02118(17) Uani 1 1 d .
Mo4 Mo -0.05289(2) 0.59731(4) 0.40807(3) 0.01756(16) Uani 1 1 d .
Mo5 Mo 0.00507(2) 0.75148(4) 0.40166(3) 0.01580(16) Uani 1 1 d .
Mo6 Mo -0.02150(3) 0.75879(5) 0.49057(3) 0.02351(18) Uani 1 1 d .
Mo7 Mo -0.11805(3) 0.75954(5) 0.38075(4) 0.02334(18) Uani 1 1 d .
Mo8 Mo 0.07969(2) 1.04961(4) 0.30561(3) 0.01504(16) Uani 1 1 d .
Mo9 Mo 0.13698(2) 1.19163(5) 0.30321(4) 0.02112(18) Uani 1 1 d .
Mo10 Mo 0.18638(2) 1.03900(5) 0.29545(3) 0.01948(17) Uani 1 1 d .
Mo11 Mo 0.18618(2) 1.06797(5) 0.41525(3) 0.01800(17) Uani 1 1 d .
Mo12 Mo 0.12164(2) 0.91348(4) 0.40444(3) 0.01538(16) Uani 1 1 d .
Mo13 Mo 0.22236(3) 0.90953(5) 0.50104(3) 0.02460(19) Uani 1 1 d .
Mo14 Mo 0.23240(2) 0.90448(5) 0.39576(4) 0.02237(18) Uani 1 1 d .
Mo15 Mo 0.0000 0.83234(6) 0.2500 0.0134(2) Uani 1 2 d S
Na1 Na 0.10316(16) 0.8309(3) 0.2525(2) 0.0478(12) Uani 1 1 d .
O1 O 0.0182(2) 0.6116(4) 0.3183(3) 0.0234(14) Uani 1 1 d .
O2 O -0.0686(2) 0.6217(4) 0.2305(3) 0.0214(13) Uani 1 1 d .
O3 O -0.0370(2) 0.5011(4) 0.3140(3) 0.0219(13) Uani 1 1 d .
O4 O -0.03500(19) 0.7246(4) 0.3219(3) 0.0190(13) Uani 1 1 d .
O5 O -0.00841(19) 0.6188(3) 0.3970(2) 0.0182(13) Uani 1 1 d .
O6 O -0.08831(19) 0.5951(3) 0.3114(2) 0.0177(13) Uani 1 1 d .
O7 O -0.1211(2) 0.4694(4) 0.2253(3) 0.0326(16) Uani 1 1 d .
O8 O -0.0669(3) 0.3703(4) 0.3222(4) 0.047(2) Uani 1 1 d .
O9 O -0.1064(3) 0.3709(4) 0.3152(3) 0.044(2) Uani 1 1 d .
O10 O -0.1452(2) 0.5058(4) 0.2980(3) 0.0246(14) Uani 1 1 d .
O11 O -0.0576(2) 0.4937(4) 0.3984(3) 0.0264(15) Uani 1 1 d .
O12 O -0.1737(2) 0.6244(5) 0.2142(3) 0.0353(17) Uani 1 1 d .
O13 O -0.1992(2) 0.6253(4) 0.2890(3) 0.0325(16) Uani 1 1 d .
O14 O -0.1358(2) 0.7306(4) 0.3044(3) 0.0234(14) Uani 1 1 d .
O15 O -0.1100(2) 0.6267(4) 0.3812(3) 0.0229(14) Uani 1 1 d .
O16 O -0.0272(2) 0.6151(4) 0.4802(3) 0.0274(15) Uani 1 1 d .
O17 O -0.0517(2) 0.7343(3) 0.4061(2) 0.0181(13) Uani 1 1 d .
O18 O 0.0531(2) 0.7334(4) 0.4067(3) 0.0230(14) Uani 1 1 d .
O19 O -0.0020(2) 0.8538(4) 0.3947(3) 0.0223(14) Uani 1 1 d .
O20 O 0.0262(2) 0.7390(4) 0.4798(3) 0.0224(14) Uani 1 1 d .
O21 O -0.0198(2) 0.8599(4) 0.4903(3) 0.0324(16) Uani 1 1 d .
O22 O 0.0243(3) 0.7309(6) 0.5674(4) 0.057(2) Uani 1 1 d .
O23 O -0.0145(3) 0.7351(5) 0.5615(4) 0.055(2) Uani 1 1 d .
O24 O -0.0831(2) 0.7475(4) 0.4616(3) 0.0309(16) Uani 1 1 d .
O25 O -0.1129(2) 0.8598(4) 0.3731(3) 0.0363(17) Uani 1 1 d .
O26 O -0.1683(2) 0.7475(4) 0.3708(3) 0.0308(16) Uani 1 1 d .
O27 O 0.03822(18) 1.0516(4) 0.3159(3) 0.0211(13) Uani 1 1 d .
O28 O 0.0556(2) 1.0413(4) 0.2334(3) 0.0222(14) Uani 1 1 d .
O29 O 0.0913(2) 1.1635(4) 0.3155(3) 0.0235(14) Uani 1 1 d .
O30 O 0.09721(19) 0.9393(3) 0.3255(2) 0.0179(13) Uani 1 1 d .
O31 O 0.13071(19) 1.0462(4) 0.3990(2) 0.0189(13) Uani 1 1 d .
O32 O 0.14299(18) 1.0693(3) 0.3181(2) 0.0171(12) Uani 1 1 d .
O33 O 0.1043(2) 1.1960(4) 0.2314(3) 0.0313(16) Uani 1 1 d .
O34 O 0.1286(3) 1.2947(5) 0.3265(4) 0.057(2) Uani 1 1 d .
O35 O 0.1644(3) 1.2950(5) 0.3242(4) 0.051(2) Uani 1 1 d .
O36 O 0.1899(2) 1.1585(4) 0.3080(3) 0.0236(14) Uani 1 1 d .
O37 O 0.1833(2) 1.1709(4) 0.4041(3) 0.0283(15) Uani 1 1 d .
O38 O 0.1478(2) 1.0341(4) 0.2245(3) 0.0307(16) Uani 1 1 d .
O39 O 0.2350(2) 1.0490(4) 0.3018(3) 0.0259(14) Uani 1 1 d .
O40 O 0.1862(2) 0.9317(4) 0.3156(3) 0.0230(14) Uani 1 1 d .
O41 O 0.22391(18) 1.0367(4) 0.3930(3) 0.0205(13) Uani 1 1 d .
O42 O 0.2193(2) 1.0530(4) 0.4883(3) 0.0296(16) Uani 1 1 d .
O43 O 0.18381(18) 0.9314(4) 0.4151(2) 0.0190(13) Uani 1 1 d .
O44 O 0.07656(19) 0.9312(4) 0.4054(3) 0.0209(13) Uani 1 1 d .
O45 O 0.12361(19) 0.8109(4) 0.3993(3) 0.0205(13) Uani 1 1 d .
O46 O 0.16343(19) 0.9298(4) 0.4834(2) 0.0212(13) Uani 1 1 d .
O47 O 0.2200(2) 0.8090(4) 0.5020(3) 0.0337(17) Uani 1 1 d .
O48 O 0.2379(3) 0.9384(6) 0.5759(3) 0.058(2) Uani 1 1 d .
O49 O 0.2746(3) 0.9330(6) 0.5739(4) 0.061(3) Uani 1 1 d .
O50 O 0.2632(2) 0.9178(4) 0.4768(3) 0.0300(16) Uani 1 1 d .
O51 O 0.2198(2) 0.8042(4) 0.3878(3) 0.0374(18) Uani 1 1 d .
O52 O 0.2764(2) 0.9123(5) 0.3921(3) 0.0371(18) Uani 1 1 d .
O53 O 0.04537(19) 0.7720(4) 0.2941(3) 0.0216(13) Uani 1 1 d .
O54 O -0.0104(2) 0.8929(4) 0.2918(3) 0.0217(13) Uani 1 1 d .
N1 N 0.1730(4) 0.4613(8) 0.4733(6) 0.087(5) Uani 1 1 d .
N2 N -0.0242(7) 0.2798(16) 0.2820(11) 0.068(8) Uani 0.50 1 d P
O1W O 0.1476(2) 0.7078(5) 0.3436(4) 0.042(2) Uani 1 1 d .
O2W O 0.1636(3) 0.6731(5) 0.4632(3) 0.051(2) Uani 1 1 d .
O3W O 0.1242(3) 0.5370(5) 0.3693(3) 0.057(3) Uani 1 1 d .
O4W O 0.0892(4) 0.5726(6) 0.4352(5) 0.074(3) Uani 1 1 d .
O5W O 0.0614(3) 1.0963(5) 0.4297(4) 0.047(2) Uani 1 1 d .
O6W O -0.0267(3) 1.1287(5) 0.3651(3) 0.052(2) Uani 1 1 d .
O7W O -0.0705(3) 0.9590(5) 0.3420(4) 0.056(3) Uani 1 1 d .
O8W O 0.0219(3) 0.9890(5) 0.4643(3) 0.050(2) Uani 1 1 d .
O9W O 0.2868(3) 1.1428(5) 0.4050(3) 0.049(2) Uani 1 1 d .
O10W O 0.2059(3) 1.1579(5) 0.2033(3) 0.050(2) Uani 1 1 d .
O11W O 0.2725(3) 1.3005(6) 0.2540(4) 0.063(3) Uani 1 1 d .
O12W O 0.1939(3) 1.3057(5) 0.2504(4) 0.047(2) Uani 1 1 d .
O13W O 0.2611(3) 1.3144(6) 0.3708(4) 0.062(3) Uani 1 1 d .
O14W O 0.0256(3) 0.4322(5) 0.4201(3) 0.0421(19) Uani 1 1 d U
O15W O 0.0895(3) 0.6466(5) 0.5737(3) 0.037(2) Uani 1 1 d .
O16W O 0.7848(3) 0.4541(6) 0.1663(4) 0.068(3) Uani 1 1 d .
O17W O 0.2264(4) 0.8006(7) 0.6275(5) 0.075(3) Uani 1 1 d .
O18W O 0.0679(8) 1.2363(9) 0.3813(9) 0.067(7) Uani 0.50 1 d P
O19W O 0.2368(6) 0.9622(10) 0.2162(8) 0.055(5) Uani 0.50 1 d PU
O20W O 0.2131(6) 1.3350(10) 0.4412(8) 0.054(4) Uani 0.50 1 d PU
O21W O 0.3223(6) 0.8980(11) 0.3379(7) 0.132(6) Uani 1 1 d .
O22W O -0.1573(9) 0.9907(13) 0.3804(11) 0.085(7) Uani 0.50 1 d P
O23W O 0.1391(7) 1.2592(17) 0.0412(7) 0.083(8) Uani 0.50 1 d P
O24W O 0.0000 0.4349(19) 0.2500 0.074(8) Uani 0.50 2 d SPU
O25W O 0.0805(10) 0.6150(18) 0.5448(14) 0.097(9) Uani 0.50 1 d PU
O26W O 0.1516(7) 1.0771(13) 0.5279(9) 0.073(6) Uani 0.50 1 d PU
O27W O -0.1111(9) 0.6484(18) 0.5115(13) 0.111(9) Uani 0.50 1 d PU
O28W O 0.0965(10) 1.1160(17) 0.0355(13) 0.114(9) Uani 0.50 1 d PU
O29W O -0.1365(11) 0.520(2) 0.4383(15) 0.130(11) Uani 0.50 1 d PU
O30W O 0.2510(10) 1.2840(17) 0.4624(12) 0.101(8) Uani 0.50 1 d PU
O31W O 0.1187(4) 1.2014(12) 0.1377(6) 0.131(6) Uani 1 1 d .
O32W O -0.0547(17) 0.415(3) 0.158(2) 0.091(15) Uani 0.25 1 d PU
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O53 Ce1 O1 77.0(2) . .
O53 Ce1 O18 77.9(2) . .
O1 Ce1 O18 71.3(2) . .
O53 Ce1 O2 70.6(2) . 2
O1 Ce1 O2 70.5(2) . 2
O18 Ce1 O2 134.6(2) . 2
O53 Ce1 O45 69.9(2) . .
O1 Ce1 O45 136.0(2) . .
O18 Ce1 O45 74.0(2) . .
O2 Ce1 O45 121.5(2) 2 .
O53 Ce1 O3W 137.5(2) . .
O1 Ce1 O3W 90.6(3) . .
O18 Ce1 O3W 136.5(3) . .
O2 Ce1 O3W 66.9(2) 2 .
O45 Ce1 O3W 133.4(3) . .
O53 Ce1 O1W 85.9(2) . .
O1 Ce1 O1W 139.2(2) . .
O18 Ce1 O1W 140.8(2) . .
O2 Ce1 O1W 69.0(2) 2 .
O45 Ce1 O1W 66.9(2) . .
O3W Ce1 O1W 77.4(3) . .
O53 Ce1 O2W 136.5(2) . .
O1 Ce1 O2W 139.1(3) . .
O18 Ce1 O2W 91.2(3) . .
O2 Ce1 O2W 134.0(2) 2 .
O45 Ce1 O2W 66.6(2) . .
O3W Ce1 O2W 77.0(3) . .
O1W Ce1 O2W 76.3(3) . .
O53 Ce1 O4W 139.1(3) . .
O1 Ce1 O4W 70.1(3) . .
O18 Ce1 O4W 69.0(3) . .
O2 Ce1 O4W 118.0(3) 2 .
O45 Ce1 O4W 120.3(3) . .
O3W Ce1 O4W 67.6(3) . .
O1W Ce1 O4W 135.0(3) . .
O2W Ce1 O4W 69.1(3) . .
O54 Ce2 O44 77.9(2) . .
O54 Ce2 O28 70.2(2) . 2
O44 Ce2 O28 135.5(2) . 2
O54 Ce2 O27 76.0(2) . .
O44 Ce2 O27 71.04(19) . .
O28 Ce2 O27 71.7(2) 2 .
O54 Ce2 O7W 87.2(3) . .
O44 Ce2 O7W 140.4(2) . .
O28 Ce2 O7W 68.8(2) 2 .
O27 Ce2 O7W 140.3(2) . .
O54 Ce2 O19 69.4(2) . .
O44 Ce2 O19 74.7(2) . .
O28 Ce2 O19 119.2(2) 2 .
O27 Ce2 O19 135.3(2) . .
O7W Ce2 O19 65.7(2) . .
O54 Ce2 O6W 137.0(2) . .
O44 Ce2 O6W 136.9(2) . .
O28 Ce2 O6W 66.8(2) 2 .
O27 Ce2 O6W 91.4(3) . .
O7W Ce2 O6W 76.7(3) . .
O19 Ce2 O6W 133.2(3) . .
O54 Ce2 O8W 135.8(2) . .
O44 Ce2 O8W 85.0(3) . .
O28 Ce2 O8W 139.4(3) 2 .
O27 Ce2 O8W 135.4(2) . .
O7W Ce2 O8W 80.6(3) . .
O19 Ce2 O8W 66.8(2) . .
O6W Ce2 O8W 81.0(3) . .
O54 Ce2 O5W 140.2(2) . .
O44 Ce2 O5W 71.7(2) . .
O28 Ce2 O5W 116.5(2) 2 .
O27 Ce2 O5W 70.4(2) . .
O7W Ce2 O5W 132.5(3) . .
O19 Ce2 O5W 123.7(2) . .
O6W Ce2 O5W 65.4(3) . .
O8W Ce2 O5W 66.5(3) . .
O36 Ce3 O13 130.9(2) . 3
O36 Ce3 O13W 87.2(3) . .
O13 Ce3 O13W 136.0(3) 3 .
O36 Ce3 O9W 76.8(2) . .
O13 Ce3 O9W 92.8(3) 3 .
O13W Ce3 O9W 73.3(3) . .
O36 Ce3 O12W 74.0(2) . .
O13 Ce3 O12W 133.3(3) 3 .
O13W Ce3 O12W 70.2(3) . .
O9W Ce3 O12W 133.7(3) . .
O36 Ce3 O10W 83.9(3) . .
O13 Ce3 O10W 73.7(3) 3 .
O13W Ce3 O10W 141.1(3) . .
O9W Ce3 O10W 139.7(3) . .
O12W Ce3 O10W 71.0(3) . .
O36 Ce3 O26 143.3(2) . 3
O13 Ce3 O26 67.7(2) 3 3
O13W Ce3 O26 68.3(3) . 3
O9W Ce3 O26 70.3(2) . 3
O12W Ce3 O26 118.8(3) . 3
O10W Ce3 O26 132.3(2) . 3
O36 Ce3 O11W 140.4(2) . .
O13 Ce3 O11W 74.6(3) 3 .
O13W Ce3 O11W 88.7(4) . .
O9W Ce3 O11W 138.6(3) . .
O12W Ce3 O11W 67.6(3) . .
O10W Ce3 O11W 75.1(3) . .
O26 Ce3 O11W 68.5(3) 3 .
O36 Ce3 O39 60.5(2) . .
O13 Ce3 O39 71.0(2) 3 .
O13W Ce3 O39 134.5(3) . .
O9W Ce3 O39 69.0(2) . .
O12W Ce3 O39 122.3(2) . .
O10W Ce3 O39 70.8(3) . .
O26 Ce3 O39 118.9(2) 3 .
O11W Ce3 O39 136.7(3) . .
O36 Ce3 Mo10 33.36(14) . .
O13 Ce3 Mo10 97.64(16) 3 .
O13W Ce3 Mo10 116.4(2) . .
O9W Ce3 Mo10 72.76(17) . .
O12W Ce3 Mo10 99.30(19) . .
O10W Ce3 Mo10 71.8(2) . .
O26 Ce3 Mo10 139.13(16) 3 .
O11W Ce3 Mo10 146.8(2) . .
O39 Ce3 Mo10 27.41(14) . .
O2 Mo1 O1 105.9(3) . .
O2 Mo1 O4 98.3(3) . .
O1 Mo1 O4 98.4(3) . .
O2 Mo1 O3 100.9(3) . .
O1 Mo1 O3 95.2(3) . .
O4 Mo1 O3 152.4(3) . .
O2 Mo1 O6 91.4(3) . .
O1 Mo1 O6 160.7(3) . .
O4 Mo1 O6 87.3(2) . .
O3 Mo1 O6 72.7(2) . .
O2 Mo1 O5 161.3(3) . .
O1 Mo1 O5 91.9(3) . .
O4 Mo1 O5 73.0(2) . .
O3 Mo1 O5 82.7(2) . .
O6 Mo1 O5 72.0(2) . .
O2 Mo1 Mo2 87.6(2) . .
O1 Mo1 Mo2 130.6(2) . .
O4 Mo1 Mo2 127.10(18) . .
O3 Mo1 Mo2 35.42(18) . .
O6 Mo1 Mo2 39.83(15) . .
O5 Mo1 Mo2 85.04(15) . .
O7 Mo2 O9 102.9(3) . .
O7 Mo2 O8 104.2(4) . .
O9 Mo2 O8 41.9(3) . .
O7 Mo2 O3 97.3(3) . .
O9 Mo2 O3 121.9(3) . .
O8 Mo2 O3 80.6(3) . .
O7 Mo2 O10 96.2(3) . .
O9 Mo2 O10 83.0(3) . .
O8 Mo2 O10 123.9(3) . .
O3 Mo2 O10 147.7(3) . .
O7 Mo2 O6 101.6(3) . .
O9 Mo2 O6 148.1(3) . .
O8 Mo2 O6 146.0(3) . .
O3 Mo2 O6 74.3(2) . .
O10 Mo2 O6 74.3(2) . .
O7 Mo2 O11 174.0(3) . .
O9 Mo2 O11 82.5(3) . .
O8 Mo2 O11 81.5(3) . .
O3 Mo2 O11 81.7(2) . .
O10 Mo2 O11 81.9(3) . .
O6 Mo2 O11 72.5(2) . .
O7 Mo2 Mo3 89.8(3) . .
O9 Mo2 Mo3 117.7(3) . .
O8 Mo2 Mo3 157.0(3) . .
O3 Mo2 Mo3 116.22(18) . .
O10 Mo2 Mo3 34.69(18) . .
O6 Mo2 Mo3 42.37(16) . .
O11 Mo2 Mo3 85.37(15) . .
O7 Mo2 Mo1 90.8(2) . .
O9 Mo2 Mo1 155.2(3) . .
O8 Mo2 Mo1 115.0(3) . .
O3 Mo2 Mo1 34.51(18) . .
O10 Mo2 Mo1 116.32(18) . .
O6 Mo2 Mo1 42.46(16) . .
O11 Mo2 Mo1 85.01(15) . .
Mo3 Mo2 Mo1 82.42(3) . .
O12 Mo3 O13 106.3(3) . .
O12 Mo3 O10 100.8(3) . .
O13 Mo3 O10 96.7(3) . .
O12 Mo3 O14 97.7(3) . .
O13 Mo3 O14 97.3(3) . .
O10 Mo3 O14 152.6(3) . .
O12 Mo3 O6 94.0(3) . .
O13 Mo3 O6 158.8(3) . .
O10 Mo3 O6 72.9(2) . .
O14 Mo3 O6 85.8(2) . .
O12 Mo3 O15 162.4(3) . .
O13 Mo3 O15 89.8(3) . .
O10 Mo3 O15 83.8(3) . .
O14 Mo3 O15 72.8(2) . .
O6 Mo3 O15 71.0(2) . .
O12 Mo3 Mo2 88.6(3) . .
O13 Mo3 Mo2 132.4(2) . .
O10 Mo3 Mo2 35.69(18) . .
O14 Mo3 Mo2 125.77(18) . .
O6 Mo3 Mo2 39.94(15) . .
O15 Mo3 Mo2 85.39(16) . .
O16 Mo4 O11 107.2(3) . .
O16 Mo4 O15 100.9(3) . .
O11 Mo4 O15 101.8(3) . .
O16 Mo4 O5 102.0(3) . .
O11 Mo4 O5 100.5(3) . .
O15 Mo4 O5 141.5(3) . .
O16 Mo4 O17 81.6(3) . .
O11 Mo4 O17 171.2(3) . .
O15 Mo4 O17 76.2(2) . .
O5 Mo4 O17 77.0(2) . .
O16 Mo4 O6 171.1(3) . .
O11 Mo4 O6 81.6(3) . .
O15 Mo4 O6 75.7(2) . .
O5 Mo4 O6 77.0(2) . .
O17 Mo4 O6 89.6(2) . .
O19 Mo5 O18 105.4(3) . .
O19 Mo5 O20 100.3(3) . .
O18 Mo5 O20 98.5(3) . .
O19 Mo5 O4 97.2(3) . .
O18 Mo5 O4 98.0(3) . .
O20 Mo5 O4 151.6(3) . .
O19 Mo5 O17 92.7(3) . .
O18 Mo5 O17 161.3(3) . .
O20 Mo5 O17 72.9(2) . .
O4 Mo5 O17 84.3(2) . .
O19 Mo5 O5 162.0(3) . .
O18 Mo5 O5 91.1(3) . .
O20 Mo5 O5 84.0(2) . .
O4 Mo5 O5 72.9(2) . .
O17 Mo5 O5 71.7(2) . .
O19 Mo5 Mo6 87.6(2) . .
O18 Mo5 Mo6 134.5(2) . .
O20 Mo5 Mo6 35.97(19) . .
O4 Mo5 Mo6 123.87(18) . .
O17 Mo5 Mo6 39.60(15) . .
O5 Mo5 Mo6 85.81(15) . .
O21 Mo6 O23 103.1(4) . .
O21 Mo6 O22 103.6(4) . .
O23 Mo6 O22 41.3(4) . .
O21 Mo6 O24 97.6(3) . .
O23 Mo6 O24 82.1(4) . .
O22 Mo6 O24 122.5(4) . .
O21 Mo6 O20 97.3(3) . .
O23 Mo6 O20 121.1(4) . .
O22 Mo6 O20 80.4(3) . .
O24 Mo6 O20 148.4(3) . .
O21 Mo6 O17 101.0(3) . .
O23 Mo6 O17 148.5(3) . .
O22 Mo6 O17 146.9(3) . .
O24 Mo6 O17 75.0(3) . .
O20 Mo6 O17 74.9(2) . .
O21 Mo6 O16 173.8(3) . .
O23 Mo6 O16 82.8(3) . .
O22 Mo6 O16 82.0(3) . .
O24 Mo6 O16 81.4(3) . .
O20 Mo6 O16 80.8(2) . .
O17 Mo6 O16 72.8(2) . .
O21 Mo6 Mo7 90.9(3) . .
O23 Mo6 Mo7 116.6(3) . .
O22 Mo6 Mo7 155.5(3) . .
O24 Mo6 Mo7 34.5(2) . .
O20 Mo6 Mo7 117.69(18) . .
O17 Mo6 Mo7 43.06(17) . .
O16 Mo6 Mo7 84.85(17) . .
O21 Mo6 Mo5 90.3(2) . .
O23 Mo6 Mo5 154.4(3) . .
O22 Mo6 Mo5 114.7(3) . .
O24 Mo6 Mo5 118.0(2) . .
O20 Mo6 Mo5 34.36(18) . .
O17 Mo6 Mo5 43.25(17) . .
O16 Mo6 Mo5 84.84(15) . .
Mo7 Mo6 Mo5 84.32(3) . .
O25 Mo7 O26 106.1(3) . .
O25 Mo7 O24 101.9(3) . .
O26 Mo7 O24 97.5(3) . .
O25 Mo7 O14 95.4(3) . .
O26 Mo7 O14 97.1(3) . .
O24 Mo7 O14 153.2(3) . .
O25 Mo7 O17 92.6(3) . .
O26 Mo7 O17 160.4(3) . .
O24 Mo7 O17 72.6(3) . .
O14 Mo7 O17 86.4(2) . .
O25 Mo7 O15 161.2(3) . .
O26 Mo7 O15 90.8(3) . .
O24 Mo7 O15 83.7(3) . .
O14 Mo7 O15 73.8(2) . .
O17 Mo7 O15 71.6(2) . .
O25 Mo7 Mo6 89.1(3) . .
O26 Mo7 Mo6 133.0(2) . .
O24 Mo7 Mo6 35.4(2) . .
O14 Mo7 Mo6 126.07(19) . .
O17 Mo7 Mo6 39.64(15) . .
O15 Mo7 Mo6 85.23(17) . .
O27 Mo8 O28 106.4(3) . .
O27 Mo8 O30 99.0(3) . .
O28 Mo8 O30 98.0(3) . .
O27 Mo8 O29 96.0(3) . .
O28 Mo8 O29 100.2(3) . .
O30 Mo8 O29 152.1(3) . .
O27 Mo8 O32 161.4(3) . .
O28 Mo8 O32 90.2(3) . .
O30 Mo8 O32 86.5(2) . .
O29 Mo8 O32 72.4(2) . .
O27 Mo8 O31 92.7(3) . .
O28 Mo8 O31 160.0(3) . .
O30 Mo8 O31 72.8(2) . .
O29 Mo8 O31 83.1(3) . .
O32 Mo8 O31 71.9(2) . .
O27 Mo8 Mo9 131.0(2) . .
O28 Mo8 Mo9 86.8(2) . .
O30 Mo8 Mo9 126.25(18) . .
O29 Mo8 Mo9 35.01(18) . .
O32 Mo8 Mo9 39.76(15) . .
O31 Mo8 Mo9 84.85(15) . .
O33 Mo9 O35 103.5(4) . .
O33 Mo9 O34 103.3(4) . .
O35 Mo9 O34 41.7(4) . .
O33 Mo9 O29 96.5(3) . .
O35 Mo9 O29 121.3(3) . .
O34 Mo9 O29 80.3(3) . .
O33 Mo9 O36 96.5(3) . .
O35 Mo9 O36 83.9(3) . .
O34 Mo9 O36 124.9(3) . .
O29 Mo9 O36 147.6(3) . .
O33 Mo9 O32 102.2(3) . .
O35 Mo9 O32 147.5(3) . .
O34 Mo9 O32 145.9(3) . .
O29 Mo9 O32 74.6(2) . .
O36 Mo9 O32 73.7(2) . .
O33 Mo9 O37 174.2(3) . .
O35 Mo9 O37 81.8(3) . .
O34 Mo9 O37 82.2(3) . .
O29 Mo9 O37 82.5(3) . .
O36 Mo9 O37 81.6(3) . .
O32 Mo9 O37 72.0(2) . .
O33 Mo9 Mo8 91.1(2) . .
O35 Mo9 Mo8 154.1(3) . .
O34 Mo9 Mo8 114.5(3) . .
O29 Mo9 Mo8 34.31(18) . .
O36 Mo9 Mo8 115.98(18) . .
O32 Mo9 Mo8 42.73(16) . .
O37 Mo9 Mo8 84.87(15) . .
O33 Mo9 Mo10 90.3(2) . .
O35 Mo9 Mo10 120.5(3) . .
O34 Mo9 Mo10 159.5(3) . .
O29 Mo9 Mo10 113.79(18) . .
O36 Mo9 Mo10 36.72(18) . .
O32 Mo9 Mo10 39.91(16) . .
O37 Mo9 Mo10 84.91(16) . .
Mo8 Mo9 Mo10 80.02(3) . .
O38 Mo10 O39 105.6(3) . .
O38 Mo10 O40 99.8(3) . .
O39 Mo10 O40 104.0(3) . .
O38 Mo10 O36 100.7(3) . .
O39 Mo10 O36 85.6(3) . .
O40 Mo10 O36 153.9(3) . .
O38 Mo10 O32 95.2(3) . .
O39 Mo10 O32 152.1(3) . .
O40 Mo10 O32 90.2(2) . .
O36 Mo10 O32 72.1(2) . .
O38 Mo10 O41 165.3(3) . .
O39 Mo10 O41 88.8(3) . .
O40 Mo10 O41 73.8(2) . .
O36 Mo10 O41 82.4(2) . .
O32 Mo10 O41 71.9(2) . .
O38 Mo10 Mo9 89.1(2) . .
O39 Mo10 Mo9 121.4(2) . .
O40 Mo10 Mo9 129.35(19) . .
O36 Mo10 Mo9 35.77(17) . .
O32 Mo10 Mo9 39.22(16) . .
O41 Mo10 Mo9 85.23(15) . .
O38 Mo10 Ce3 103.2(2) . .
O39 Mo10 Ce3 44.3(2) . .
O40 Mo10 Ce3 144.99(19) . .
O36 Mo10 Ce3 41.81(17) . .
O32 Mo10 Ce3 113.36(16) . .
O41 Mo10 Ce3 88.76(15) . .
Mo9 Mo10 Ce3 77.29(2) . .
O37 Mo11 O42 106.8(3) . .
O37 Mo11 O31 101.4(3) . .
O42 Mo11 O31 102.4(3) . .
O37 Mo11 O41 101.1(3) . .
O42 Mo11 O41 101.2(3) . .
O31 Mo11 O41 140.8(3) . .
O37 Mo11 O43 171.2(3) . .
O42 Mo11 O43 81.9(3) . .
O31 Mo11 O43 76.8(2) . .
O41 Mo11 O43 76.1(2) . .
O37 Mo11 O32 80.9(3) . .
O42 Mo11 O32 172.2(3) . .
O31 Mo11 O32 76.7(2) . .
O41 Mo11 O32 75.8(2) . .
O43 Mo11 O32 90.4(2) . .
O44 Mo12 O45 105.1(3) . .
O44 Mo12 O46 96.8(3) . .
O45 Mo12 O46 101.3(3) . .
O44 Mo12 O30 98.5(3) . .
O45 Mo12 O30 97.9(3) . .
O46 Mo12 O30 151.3(3) . .
O44 Mo12 O43 160.7(3) . .
O45 Mo12 O43 93.3(3) . .
O46 Mo12 O43 73.2(2) . .
O30 Mo12 O43 84.6(2) . .
O44 Mo12 O31 90.9(3) . .
O45 Mo12 O31 162.5(3) . .
O46 Mo12 O31 83.4(2) . .
O30 Mo12 O31 72.2(2) . .
O43 Mo12 O31 71.8(2) . .
O44 Mo12 Mo13 132.8(2) . .
O45 Mo12 Mo13 88.1(2) . .
O46 Mo12 Mo13 36.06(18) . .
O30 Mo12 Mo13 124.72(18) . .
O43 Mo12 Mo13 40.09(15) . .
O31 Mo12 Mo13 86.04(15) . .
O47 Mo13 O48 102.6(4) . .
O47 Mo13 O49 102.4(4) . .
O48 Mo13 O49 42.5(4) . .
O47 Mo13 O46 96.6(3) . .
O48 Mo13 O46 81.2(3) . .
O49 Mo13 O46 123.0(3) . .
O47 Mo13 O50 97.5(3) . .
O48 Mo13 O50 123.1(3) . .
O49 Mo13 O50 81.5(3) . .
O46 Mo13 O50 147.9(3) . .
O47 Mo13 O43 100.9(3) . .
O48 Mo13 O43 147.7(3) . .
O49 Mo13 O43 148.6(3) . .
O46 Mo13 O43 74.3(2) . .
O50 Mo13 O43 74.8(2) . .
O47 Mo13 O42 173.5(3) . .
O48 Mo13 O42 83.0(3) . .
O49 Mo13 O42 84.0(4) . .
O46 Mo13 O42 80.8(2) . .
O50 Mo13 O42 82.0(3) . .
O43 Mo13 O42 72.7(2) . .
O47 Mo13 Mo12 89.3(2) . .
O48 Mo13 Mo12 115.6(3) . .
O49 Mo13 Mo12 156.7(3) . .
O46 Mo13 Mo12 34.43(17) . .
O50 Mo13 Mo12 117.25(19) . .
O43 Mo13 Mo12 42.86(16) . .
O42 Mo13 Mo12 85.15(16) . .
O47 Mo13 Mo14 91.3(3) . .
O48 Mo13 Mo14 156.0(3) . .
O49 Mo13 Mo14 115.7(3) . .
O46 Mo13 Mo14 116.94(17) . .
O50 Mo13 Mo14 34.26(19) . .
O43 Mo13 Mo14 42.84(17) . .
O42 Mo13 Mo14 84.65(16) . .
Mo12 Mo13 Mo14 83.61(3) . .
O52 Mo14 O51 105.5(4) . .
O52 Mo14 O50 96.6(3) . .
O51 Mo14 O50 101.9(3) . .
O52 Mo14 O40 99.0(3) . .
O51 Mo14 O40 94.2(3) . .
O50 Mo14 O40 153.6(3) . .
O52 Mo14 O43 161.4(3) . .
O51 Mo14 O43 91.7(3) . .
O50 Mo14 O43 72.7(2) . .
O40 Mo14 O43 86.2(2) . .
O52 Mo14 O41 92.5(3) . .
O51 Mo14 O41 159.8(3) . .
O50 Mo14 O41 84.6(3) . .
O40 Mo14 O41 73.7(2) . .
O43 Mo14 O41 71.7(2) . .
O52 Mo14 Mo13 132.0(3) . .
O51 Mo14 Mo13 89.1(3) . .
O50 Mo14 Mo13 35.5(2) . .
O40 Mo14 Mo13 125.69(18) . .
O43 Mo14 Mo13 39.45(15) . .
O41 Mo14 Mo13 85.34(16) . .
O53 Mo15 O53 109.8(4) 2 .
O53 Mo15 O54 109.1(3) 2 .
O53 Mo15 O54 109.5(3) . .
O53 Mo15 O54 109.5(3) 2 2
O53 Mo15 O54 109.1(3) . 2
O54 Mo15 O54 109.8(4) . 2
O4 Na1 O30 122.6(2) 2 .
O4 Na1 O1W 92.7(2) 2 .
O30 Na1 O1W 92.1(2) . .
O4 Na1 O14 73.3(2) 2 2
O30 Na1 O14 163.8(3) . 2
O1W Na1 O14 83.6(2) . 2
Mo1 O1 Ce1 149.1(3) . .
Mo1 O2 Ce1 154.7(3) . 2
Mo1 O3 Mo2 110.1(3) . .
Mo1 O4 Mo5 114.9(3) . .
Mo1 O4 Na1 122.7(3) . 2
Mo5 O4 Na1 120.6(3) . 2
Mo4 O5 Mo5 111.4(3) . .
Mo4 O5 Mo1 110.8(3) . .
Mo5 O5 Mo1 92.0(2) . .
Mo2 O6 Mo3 97.7(2) . .
Mo2 O6 Mo1 97.7(2) . .
Mo3 O6 Mo1 150.9(3) . .
Mo2 O6 Mo4 100.3(2) . .
Mo3 O6 Mo4 101.2(2) . .
Mo1 O6 Mo4 100.2(2) . .
O9 O8 Mo2 68.3(5) . .
O8 O9 Mo2 69.8(5) . .
Mo3 O10 Mo2 109.6(3) . .
Mo4 O11 Mo2 105.5(3) . .
Mo3 O13 Ce3 151.3(4) . 3_445
Mo7 O14 Mo3 113.4(3) . .
Mo7 O14 Na1 118.2(3) . 2
Mo3 O14 Na1 124.3(3) . 2
Mo4 O15 Mo7 112.2(3) . .
Mo4 O15 Mo3 111.8(3) . .
Mo7 O15 Mo3 92.4(2) . .
Mo4 O16 Mo6 105.5(3) . .
Mo6 O17 Mo7 97.3(2) . .
Mo6 O17 Mo5 97.1(2) . .
Mo7 O17 Mo5 153.6(3) . .
Mo6 O17 Mo4 100.2(2) . .
Mo7 O17 Mo4 99.6(2) . .
Mo5 O17 Mo4 99.5(2) . .
Mo5 O18 Ce1 149.3(3) . .
Mo5 O19 Ce2 155.6(3) . .
Mo5 O20 Mo6 109.7(3) . .
O23 O22 Mo6 69.1(6) . .
O22 O23 Mo6 69.7(5) . .
Mo7 O24 Mo6 110.1(3) . .
Mo7 O26 Ce3 148.8(4) . 3_445
Mo8 O27 Ce2 148.6(3) . .
Mo8 O28 Ce2 152.0(3) . 2
Mo8 O29 Mo9 110.7(3) . .
Mo8 O30 Mo12 114.5(3) . .
Mo8 O30 Na1 122.9(3) . .
Mo12 O30 Na1 121.5(3) . .
Mo11 O31 Mo8 112.0(3) . .
Mo11 O31 Mo12 111.0(3) . .
Mo8 O31 Mo12 92.6(2) . .
Mo9 O32 Mo10 100.9(2) . .
Mo9 O32 Mo8 97.5(2) . .
Mo10 O32 Mo8 148.0(3) . .
Mo9 O32 Mo11 100.3(2) . .
Mo10 O32 Mo11 103.0(2) . .
Mo8 O32 Mo11 99.2(2) . .
O35 O34 Mo9 68.8(5) . .
O34 O35 Mo9 69.5(5) . .
Mo9 O36 Mo10 107.5(3) . .
Mo9 O36 Ce3 146.4(3) . .
Mo10 O36 Ce3 104.8(3) . .
Mo11 O37 Mo9 106.8(3) . .
Mo10 O39 Ce3 108.3(3) . .
Mo10 O40 Mo14 114.7(3) . .
Mo11 O41 Mo14 112.2(3) . .
Mo11 O41 Mo10 109.3(3) . .
Mo14 O41 Mo10 92.1(2) . .
Mo11 O42 Mo13 105.3(3) . .
Mo13 O43 Mo12 97.0(2) . .
Mo13 O43 Mo14 97.7(2) . .
Mo12 O43 Mo14 152.8(3) . .
Mo13 O43 Mo11 100.0(2) . .
Mo12 O43 Mo11 100.0(2) . .
Mo14 O43 Mo11 99.7(2) . .
Mo12 O44 Ce2 150.8(3) . .
Mo12 O45 Ce1 155.1(3) . .
Mo12 O46 Mo13 109.5(3) . .
O49 O48 Mo13 68.8(5) . .
O48 O49 Mo13 68.7(5) . .
Mo14 O50 Mo13 110.3(3) . .
Mo15 O53 Ce1 159.6(4) . .
Mo15 O54 Ce2 157.9(3) . .
Ce1 O1W Na1 103.9(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ce1 O53 2.443(6) .
Ce1 O1 2.490(6) .
Ce1 O18 2.510(6) .
Ce1 O2 2.513(6) 2
Ce1 O45 2.529(6) .
Ce1 O3W 2.540(8) .
Ce1 O1W 2.555(7) .
Ce1 O2W 2.558(7) .
Ce1 O4W 2.622(9) .
Ce2 O54 2.447(6) .
Ce2 O44 2.494(6) .
Ce2 O28 2.509(6) 2
Ce2 O27 2.524(6) .
Ce2 O7W 2.528(7) .
Ce2 O19 2.533(6) .
Ce2 O6W 2.548(7) .
Ce2 O8W 2.552(7) .
Ce2 O5W 2.579(8) .
Ce3 O36 2.447(6) .
Ce3 O13 2.476(7) 3
Ce3 O13W 2.511(9) .
Ce3 O9W 2.526(8) .
Ce3 O12W 2.538(8) .
Ce3 O10W 2.552(8) .
Ce3 O26 2.568(7) 3
Ce3 O11W 2.607(8) .
Ce3 O39 2.609(7) .
Ce3 Mo10 3.5481(9) .
Mo1 O2 1.729(6) .
Mo1 O1 1.742(6) .
Mo1 O4 1.923(6) .
Mo1 O3 1.924(6) .
Mo1 O6 2.174(6) .
Mo1 O5 2.271(6) .
Mo1 Mo2 3.1905(10) .
Mo2 O7 1.699(7) .
Mo2 O9 1.906(8) .
Mo2 O8 1.925(8) .
Mo2 O3 1.969(6) .
Mo2 O10 1.972(6) .
Mo2 O6 2.062(6) .
Mo2 O11 2.424(7) .
Mo2 Mo3 3.1832(11) .
Mo3 O12 1.721(7) .
Mo3 O13 1.734(7) .
Mo3 O10 1.923(6) .
Mo3 O14 1.953(6) .
Mo3 O6 2.165(6) .
Mo3 O15 2.273(7) .
Mo4 O16 1.737(6) .
Mo4 O11 1.745(6) .
Mo4 O15 1.877(6) .
Mo4 O5 1.880(6) .
Mo4 O17 2.288(6) .
Mo4 O6 2.290(6) .
Mo5 O19 1.724(6) .
Mo5 O18 1.734(6) .
Mo5 O20 1.909(6) .
Mo5 O4 1.946(6) .
Mo5 O17 2.200(6) .
Mo5 O5 2.260(6) .
Mo5 Mo6 3.1849(11) .
Mo6 O21 1.689(7) .
Mo6 O23 1.924(9) .
Mo6 O22 1.931(9) .
Mo6 O24 1.963(7) .
Mo6 O20 1.987(6) .
Mo6 O17 2.046(6) .
Mo6 O16 2.412(7) .
Mo6 Mo7 3.1809(12) .
Mo7 O25 1.712(7) .
Mo7 O26 1.736(6) .
Mo7 O24 1.917(7) .
Mo7 O14 1.943(7) .
Mo7 O17 2.190(6) .
Mo7 O15 2.237(6) .
Mo8 O27 1.720(6) .
Mo8 O28 1.727(6) .
Mo8 O30 1.930(6) .
Mo8 O29 1.935(6) .
Mo8 O32 2.199(6) .
Mo8 O31 2.241(6) .
Mo8 Mo9 3.2125(10) .
Mo9 O33 1.695(7) .
Mo9 O35 1.923(8) .
Mo9 O34 1.932(9) .
Mo9 O29 1.970(6) .
Mo9 O36 1.973(6) .
Mo9 O32 2.072(6) .
Mo9 O37 2.408(7) .
Mo9 Mo10 3.2188(11) .
Mo10 O38 1.704(7) .
Mo10 O39 1.721(6) .
Mo10 O40 1.881(6) .
Mo10 O36 2.018(6) .
Mo10 O32 2.103(6) .
Mo10 O41 2.306(6) .
Mo11 O37 1.739(7) .
Mo11 O42 1.742(7) .
Mo11 O31 1.878(6) .
Mo11 O41 1.903(6) .
Mo11 O43 2.282(6) .
Mo11 O32 2.292(6) .
Mo12 O44 1.716(6) .
Mo12 O45 1.723(6) .
Mo12 O46 1.905(6) .
Mo12 O30 1.941(6) .
Mo12 O43 2.176(6) .
Mo12 O31 2.260(6) .
Mo12 Mo13 3.1755(11) .
Mo13 O47 1.682(7) .
Mo13 O48 1.928(9) .
Mo13 O49 1.929(9) .
Mo13 O46 1.983(6) .
Mo13 O50 1.988(7) .
Mo13 O43 2.061(6) .
Mo13 O42 2.415(7) .
Mo13 Mo14 3.2139(12) .
Mo14 O52 1.699(7) .
Mo14 O51 1.720(7) .
Mo14 O50 1.929(7) .
Mo14 O40 1.994(6) .
Mo14 O43 2.205(6) .
Mo14 O41 2.225(6) .
Mo15 O53 1.752(6) 2
Mo15 O53 1.752(6) .
Mo15 O54 1.759(6) .
Mo15 O54 1.759(6) 2
Na1 O4 2.839(8) 2
Na1 O30 2.853(7) .
Na1 O1W 2.980(10) .
Na1 O14 3.011(8) 2
O2 Ce1 2.513(6) 2
O4 Na1 2.839(8) 2
O8 O9 1.369(12) .
O13 Ce3 2.476(7) 3_445
O14 Na1 3.011(8) 2
O22 O23 1.359(13) .
O26 Ce3 2.568(7) 3_445
O28 Ce2 2.509(6) 2
O34 O35 1.371(12) .
O48 O49 1.398(13) .
O15W O25W 0.87(3) .
O20W O30W 1.46(3) .
